**POLITECNICO DI MILANO **

### Facoltà di Ingegneria Meccanica

### Master of Science in

### Mechanical Engineering

**Application of Li-ion cell ageing models **

**on automotive electrical propulsion cells**

### Supervisor: Prof. Francesco Braghin

### Co-supervisor: Davide Tarsitano; Ferdinando Mapelli

**MSc Thesis of: **

**Zhi Zhang ID. 780987 **

**CONTENT **

List of Figures ... 5

List of Tables ... 9

*Abstract: ... 10*

1. Introduction and Research Background ... 13

1.1 Outline of the thesis ... 13

1.2 EVs and EVBs background ... 15

1.3 Comparison between batteries ... 16

1.4 Important parameters ... 18

1.4.1 DOD and SOC Definition ... 19

1.4.2 Battery Life Definition ... 19

1.4.3 Efficiency ... 20

2. Literature Review ... 21

2.1 Reasons for aging ... 21

2.2 Aging Effect ... 22

2.2.1 Electrolyte ... 22

2.2.2 Negative electrode (Cathode) ... 23

2.2.3 Positive electrode (Anode) ... 24

2.3 Aging Models ... 25

2.3.1 Resistance Increasing in ECM ... 25

2.3.2 Aging Detecting From Electrochemical Impedance Spectroscopy ... 27

2.3.3 Calendar Aging Model ... 33

2.3.4 Cycle Life Aging Model ... 36

2.3.5 Shepherd Empirical Model ... 41

2.4 Battery Life Prediction from Aging ... 45

2.4.1 First Method (based on Resistance Growth)... 45

2.5 International Standard ... 51

2.5.1 Life Testing ... 51

2.5.2 Maximum allowable deviations ... 52

2.5.3 Intended Use ... 53

2.5.4 Failure Modes ... 54

2.6 Capacity Fade result from small format batteries ... 55

2.6.1 Small Size Li-Fe battery ... 55

2.6.2 LiCo2/C Battery ... 56

2.6.3 10Ah LiFePO4-based Li-ion batteries ... 58

3. Experimental Set-up ... 62

3.1 Test Bench for test ... 62

3.1.1 Battery Specification ... 65

3.1.2 Power Supply-Charge system ... 69

3.1.3 Discharge system ... 72

3.1.4 BNC Adapter for Digital and Analog Signals ... 76

3.2 Software Structure ... 79

3.3 Experimental Environment and Challenges ... 83

4. Modeling and Data Analysis ... 84

4.1 Cycling Result ... 84

4.2 Data Analysis ... 87

4.3 Numerical Models for Fitting and Life prediction ... 91

4.3.1 First Cycling Model (based on Ah-throughput) ... 92

4.3.2 Second Cycling Model (based on capacitance) ... 96

4.4. Discussion of the Results ... 98

Acknowledgements ... 108

Appendix A-Main Program ... 109

Appendix B- Monitoring ... 116

Appendix C- Data Analysis Program ... 118

**List of Figures **

FIGURE 1 ELECTRIC VEHICLE ... 15

FIGURE 2 CHANGES AT THE ANODE/ELECTROLYTE INTERFACE ... 23

FIGURE 3 SURFACE FILM FORMATION ON GRAPHITE ELECTRODES ... 24

FIGURE 4 A LISTING OF THE MAJOR DYNAMIC PROCESSES IN BATTERIES AND THEIR AVERAGE TIME CONSTANTS... 25

FIGURE 5 THE RLC EQUIVALENT CIRCUIT NEEDED TO MODEL DIFFUSION EFFECTS ... 26

FIGURE 6 EQUIVALENT CIRCUIT OF 1ST ORDER RANDLE MODEL ... 27

FIGURE 7 MATHEMATIC MODEL OF THE FIRST ORDER OF THE IMPEDANCE ... 29

FIGURE 8 NYQUIST DIAGRAM OF THE WARBURG IMPEDANCE ... 30

FIGURE 9 BODE PLOT OF THE WARBURG IMPEDANCE ... 30

FIGURE 10 ECM WITH WARBURG IMPEDANCE ... 31

FIGURE 11 NYQUIST DIAGRAM OF THE SECOND ORDER WITHOUT WARBURG IMPEDANCE ... 32

FIGURE 12 MODEL PREDICTIONS FOR THE CAPACITY LOSS AFTER A 10-YEAR STORAGE PERIOD AT DIFFERENT SOC FOR THE THREE CITIES ... 34

FIGURE 13 CAPACITY LOSS PREDICTIONS AS A FUNCTION OF THE SOC OF STORAGE IN DUBAI ... 34

FIGURE 14 SEI RESISTANCE INCREASE PREDICTIONS AS A FUNCTION OF THE SOC OF STORAGE IN DUBAI ... 35

FIGURE 15 TYPICAL DISCHARGE CURVE TREND DURING CAPACITANCE MEASUREMENT 36 FIGURE 16 CAPACITANCE RETENTION TRENDS AS A FUNCTION OF SQUARE ROOT OF NUMBER OF CYCLES. ... 37

FIGURE 19 FITTING PLOT... 40

FIGURE 20 DISCHARGE VOLTAGE VARIATION FOR 4 STATES OF AGEING ... 42

FIGURE 21 VARIATION OF DISCHARGE RESISTANCE FOR 4 STATES OF AGING ... 42

FIGURE 22 CHARGE VOLTAGE VARIATION FOR 4 STATES OF AGEING ... 43

FIGURE 23 CHARGE VOLTAGE VARIATION FOR 4 STATES OF AGEING ... 43

FIGURE 24 EXAMPLE OF LIFE PREDICTION USING METHOD 1 AT 3500 AMP HOURS ... 46

FIGURE 25 PREDICTION OF THE LIFE FROM THE RESISTANCE ... 47

FIGURE 26 EXAMPLES OF CYCLE LIFE PREDICTION ... 49

FIGURE 27 SIMULATION OF CYCLE-LIFE PREDICTION MODEL AND EXPERIMENTAL DATA ... 50

FIGURE 28 CAPACITY RETENTION AT 60 ◦C AND A DISCHARGE RATE OF C/2 PLOTTED AS A FUNCTION OF CYCLE NUMBER, DATA SHOWN FOR DIFFERENT DOD [34] ... 55

FIGURE 29 CAPACITY RETENTION AT 60 .C AND A DISCHARE RATE OF C/2 PLOTTED AS A FUNCTION OF TIME (DAYS) ... 56

FIGURE 30 EXAMPLE OF CAPACITY EVOLUTIONS DURING 100% DOD CYCLING. ... 57

FIGURE 31 (A) VOLTAGE.CAPACITY CURVES FOR CELL L IN THE FIRST 15 CYCLES AT 25 CELSIUS. (B) VOLTAGE.CAPACITY CURVES FOR CELL P IN THE FIRST 5 CYCLES AT 25 CELSIUS... 59

FIGURE 32 (A) CAPACITY LOSS WITH CYCLE NUMBER FOR BOTH CELLS AND (B) EVOLUTION OF THE V VS. Q CURVES FOR CELL L. ... 60

FIGURE 33 INITIAL AND FINAL C/10 CYCLES IN THE LIFE CYCLE TEST OF CELL L AT 25 C 61 FIGURE 34 BATTERY TEST BENCH ... 62

FIGURE 35 CONNECTION DURING CHARGING ... 63

FIGURE 36 CONNECTION DURING DISCHARGING ... 64

FIGURE 37 BATTERY MODEL: TS-LFP60AHA(A) [25] ... 65

FIGURE 38 DISCHARGE CURVE UNDER NORMAL TEMPERATURE ... 66

FIGURE 39 BATTERY’S STORAGE CHARACTERISTIC CURVE IN NORMAL TEMPERATURE . 67 FIGURE 40 BATTERY’S DISCHARGE CURVE UNDER DIFFERENT TEMPERATURES ... 67

NORMAL TEMPERATURE ... 68

FIGURE 42 DIFFERENT BUTTONS ON THE PANEL OF POWER SUPPLY ... 69

FIGURE 43 SCHEMATIC OF A SWITCH-MODE DC POWER SUPPLY ... 70

FIGURE 44 PULSE-WIDTH MODULATOR: (A) BLOCK DIAGRAM; (B) COMPARATOR SIGNALS ... 71

FIGURE 45 DISCHARGE SYSTEM... 72

FIGURE 46 SPECIFICATION OF THE HEAT-SINK ... 73

FIGURE 47 STRUCTURE OF MOSFET ... 74

FIGURE 48 OUTPUT CHARACTERISTICS OF THE MOSFET ... 74

FIGURE 49 THERMAL RESISTOR STRUCTURE OF THE DISCHARGE SYSTEM ... 75

FIGURE 50 BNC-2110 ... 76

FIGURE 51 ANALOG INPUT OF THE BNC ADAPTER ... 77

FIGURE 52 ANALOG OUTPUT OF THE BNC ADAPTER ... 78

FIGURE 53 PARAMETERS DEFINITION... 79

FIGURE 54 LOGICAL CIRCUIT FOR ONE CYCLE ... 80

FIGURE 55 LOGICAL CYCLE FOR MONITORING ... 81

FIGURE 56 CURRENT STABILIZATION DURING DISCHARGING BY ANALOG OUTPUT ... 82

FIGURE 57 VOLTAGE VARIATION DURING ONE CYCLE ... 84

FIGURE 58 CURRENT VARIATION DURING ONE CYCLE ... 85

FIGURE 59 THE TEMPERATURE OF THE HEAT SINK AND BATTERY ... 86

FIGURE 60 CAPACITY RETENTION IN THE FIRST 160 CYCLES ... 88

FIGURE 61 DISCHARGE CURVE BETWEEN FIRST 160 CYCLES ... 88

FIGURE 62 DECREASING OF THE CYCLE TIME ... 89

FIGURE 63 BATTERY EFFICIENCY ... 90

FIGURE 69 VOLTAGE CHANGE WITH TIME ... 96

FIGURE 70 COMPARISON BETWEEN SECOND AGING MODEL AND REAL VALUE ... 97

FIGURE 71 CAPACITY AS A FUNCTION OF THE CYCLE NUMBER... 98

**List of Tables **

TABLE 1 GENERAL BATTERY DIFFERENCES [14] ... 17

TABLE 2 DEVIATIONS OF THE TEST PROCEDURE... 52

TABLE 3 INTENDED USE OF BATTERY [3] ... 53

TABLE 4 DIFFERENT KINDS OF FAILURE MODES ... 54

TABLE 5 SPECIFICATION OF THE BATTERY ... 65

TABLE 6 ELECTRIC PARAMETERS OF CHARGE AND DISCHARGE ... 66

TABLE 7 CHANNELS FOR ANALOG INPUT ... 77

TABLE 8 SIGNAL CONVERSION ... 78

**Abstract: **

**Abstract:**

Nowadays power is a very important characteristic for the vehicle and large-capacity batteries can produce higher power for the electrical vehicle in which the speed or the maximum load of the electrical vehicle will be increased absolutely. But most lithium-ion batteries are produced in small format with a capacity range from 100mA to 10A. They are applied in daily use such as cellphone and very few large format lithium-ion batteries have been researched. With the increasing demand of the electrical vehicles, large-capacity batteries are becoming more and more accepted by car-marking factories.

The extensive use of batteries in hybrid electric vehicles (HEVs) today requires establishing an accurate model of battery aging and life. During a battery’s lifetime, its performance slowly deteriorates because of the degradation of its electrochemical constituents, they experience power and energy fade associated with impedance rise and capacity loss, respectively. Capacity decrease and power fading do not originate from one single cause, but from a number of various processes and their interactions. Moreover, most of these processes cannot be studied independently and occur at similar timescales, complicating the investigation of ageing mechanisms. Identification of key aging parameters in lithium ion battery models can validate degradation hypotheses and provide a foundation for State of Health (SOH) estimation. Battery manufacturers usually provide aging data that will show this degradation. However the data they provide result from steady state tests, in which the battery is discharged and charged thousands of times with constant current profiles (or cycles). The current and the Depth of Discharge (DOD) in the vehicles will depend completely on the real application. Using these data many aging models have been developed that relate the maximum number of battery cycles to the DOD of the current profile used.

applications. Most of Li-ion ageing mechanisms have been experimentally identified and described in literature. Nevertheless, Li-ion ageing mechanisms are complex and can interact with each other resulting in different evolution shapes for capacity loss and power fade. Battery aging and degradation often encounter multiple complex and coupled physical–chemical processes in complicated operating conditions, including dynamic duty cycles, temperature/thermal effects, time between operations, and other environmental factors. To quantify aging and degradation effect accurately is not a simple task either. Even if a vigorous test plan can reveal how much capacity is lost in a life cycle test, the result is insufficient to either provide detailed information on degradation mechanism or predict how much loss will occur under a different regime.

This thesis has performed a Life Cycle Assessment (LCA) of a 60Ah lithium-ion (TS-LFP60AHA (A)) battery which is expected as the power source for hybrid electrical vehicles (HEVs) or full electrical vehicles (FEVs). The simulation tool MATLAB is employed to examine the behaviors of batteries and control the running of other electrical devices. To complete the test, a discharge-charge system will be designed to perform the cycling. The test bench will include battery charger, discharge system, data acquisition system, battery and computer. All the cycles will be in the constant-current (CC) situation. The stations assembled can charge and discharge the battery automatically. At the end of each cycle, test parameters (time, temperature, Voltage, current) will be saved in the computer with the name of the cycle number. The effects of test parameters were investigated and described in the following steps.

Several battery models are built to simulate the behavior of the battery and predict battery performance of cycles. The increasing resistance is widely accepted as a judgment for the aging of battery. From the trend of the discharge curve, the dynamic equivalent circuit model can be built, and the increasing resistance of the battery can be

Plot, data collected in the EIS test can reflect that the curve of the impedance respected frequency becomes narrow. In my work, capacity and capacitance analysis are used to detect and predict the phenomenon of aging. During aging, capacity fade can be measured easily and the capacitance is inverse proportional to the slope of the discharge curve. So the model can be built easily and reflect directly the trend of the aging. The models are validated through comparison with real datasheet performance and with experimental data. After finishing building the models, these models will be used to predict the life of the battery by assuming a suitable end of life (80% of the initial capacity).

Most numerical models are built based on the small size lithium-ion batteries and my work is applying these models on the automotive electrical propulsion cells which have a higher capacity. In this scenario, various studies have attempted at investigating the effects of current/power demand and cycle life, as well as estimating the residual life of the batter. A set of computing processes are running concurrently to address power capability, efficiency of the battery, and capacity retention, which are represented by cumulative Ah-throughput. The objective of this project is to utilize data originally collected with the intent of analyzing aging of the high capacity battery to create an algorithm for predicting capacity retention for the purpose of predicting high-capacity battery life. The battery life predictions made by this algorithm should be reasonably accurate. Moreover, large amount of data collected in this the experiment can be regarded as the reference of the following experiments. Following tests will base on the influence of the temperature, evaluation of mechanical stress and vibration on battery behavior and life internal stress. This work will bring a good start for the research of lithium-ion for electrical vehicles in Polytechnic of Milan.

**1. Introduction and Research Background **

**1.1 Outline of the thesis **

In the first chapter, a general introduction of the electrification of transportation was given in addition to some information on different types of battery applications. After comparison of all the type of batteries, we show the reason for study on Li-ion battery. At the end of the first chapter, the important parameters (SOC, DOD, Life Definition and Efficiency) of Li-ion battery are discussed generally.

In Chapter 2, we show the research aim, aging phenomenon, as well as the influence of aging on the battery capacity and internal resistance. From the point of the chemistry, we explain the change of the cathode, anode, and the electrolyte of the battery during aging. Furthermore, the factors which have influence on the aging and life prediction from aging were also given. A brief literature review introducing the model and methodologies was given. For example, aging detection from the equivalent circuit model and electrochemical impedance spectroscopy, calendar aging and Shepherd empirical model. Some boundary condition and international standard of experiment are also introduced in the second chapter.

In the third chapter, we present the battery experimentation hardware and software structure as well as described some of the challenges in battery testing. The battery testing systems (charger, discharger, data acquisition system, and computer) that were described are used for the battery model coefficient identification which was used in later chapters to schedule the coefficients on the single cell battery models. The work that was done to develop the testing stations is believed to be a contribution in and of it and is thus archived in this thesis.

second part, we derived an analytical solution to the battery cell models to define the trend of the battery. 2 numerical models which based on the capacitance and capacity are built to fit for the data known. From the result of the fitting we can have a better understanding that whether the models are suitable for the large-capacity cells. With the built models residual life can be predicted and numbers of cycles needed to reach the end of life (EOF).

**1.2 EVs and EVBs background **

As part of the efforts to control anthropogenic greenhouse gas emissions, the replacement of internal combustion engine vehicles by electric vehicles (EV) stirs much scientific, political, and public interest. Depending on the electricity mix used, these vehicles harbor the potential for substantial emission reductions. In these automotive applications, batteries are capable of delivering tens or hundreds of kilowatts, hence necessitating large battery packs composed of multiple series strings of cells, and often involve multiple strings in parallel to increase the pack capacity as well as to decrease the aging severity of the current seen by each cell. The present study investigates several Li-ion batteries and highlights their environmental tradeoffs.

**1.3 Comparison between batteries **

Lithium-ion batteries will play an important role in our mobility because of various advantages over other battery technologies such as the high specific energy and the high specific power, which are very important for HEV and FEV applications. In spite of these advantages there are some improvements (cycle life, calendar life and high degree of the safety) needed in order to make the lithium-ion technique more competitive in particular in terms of costs and lifetime. The ability to predict the lifetime of batteries is essential for the market introduction of lithium batteries in the electric vehicle market. But this key challenge is very complex because in this electrochemical system a number of aging processes take place parallel due to different stress factors which are caused by the varied operation conditions of the battery related to the drivers requirements.

Battery types Advantages Disadvantages Lead - Acid Can be designed for high power

Inexpensive Safe

Reliable

Poor Cold temperature

Performance

Short Calendar and Cycle Life

Nickel- Cadmium

High Specific Energy Good Cycle life compared with lead acid

Does not deliver sufficient power

Nickel-Metal Hydride

Reasonable Specific Energy Reasonable Specific Power

Much longer cycle life than lead acid Safe

Abuse-tolerant

High Cost

Heat Generation at High Temperatures

Low cell efficiency

Need to control Hydrogen Losses

Lithium Ion High Specific Energy High Specific Power High Energy Efficiency

Good High temperature performance Low Self-Discharge

Needs Improvement in: Calendar and Cycle life Abuse Tolerance Acceptable Cost

Higher degree of Battery safety Lithium

Polymer

High Specific Energy

Has potential in providing high specific power

Safe

Good Cycle and Calendar Life

Only viable if:

The cost is lower dramatically Specific Power is increased

**1.4 Important parameters **

In spite of intensive investigations on various positive and negative electrode chemistries, these aging phenomena are not yet well understood nor quantified, and the combined impacts of temperature (T), state-of-charge (SOC), depth of discharge (DOD), and current intensity (I) still remain difficult to quantify and manage. Accurate estimation of batteries life is also a great challenge in particular for lithium-ion batteries in traction applications because these batteries experience a very irregular pattern of charge and discharge cycles depending on the driver’s driving and recharging habits. The requirements of the driver (power and energy demand) determine the operating conditions of the battery like current and voltage. But also other factors like the temperature distribution within the battery, the depth of discharge (DOD) and the state of charge (SOC) of the battery must be taken into account in the lifetime estimation. These operating conditions determine the stress factors which induce the aging and the rate of aging. A successful lifetime prediction requires knowledge of the aging processes, the stress factors and their relationships.

**1.4.1 DOD and SOC Definition **

DOD is defined as the amount of Amp-hours (Ahs) removed from a battery cell expressed as a percentage of the rated capacity. DOD is the opposite of State of Charge (SOC). For example, the removal of 25 Ah from a fully charged 100 Ah rated battery results in a 25% depth of discharge. Extensive research has been done in trying to relate the cycle life of a battery to the DOD the cycle achieves [19].

Assuming the cell to be fully charged at the time t=0, the cell capacity is 𝑄𝐶, the extracted

charge, 𝑄𝑒is defined as:

𝑄_{𝑒}(𝑡) = ∫ 𝐼(𝜏)𝑡

0

𝑑𝜏 (1)

The State of charge (SOC) is:

SoC = 1 −𝑄𝑒

𝑄_{𝑐} (2)
The Depth of Discharge (DOD) is:

DoD =𝑄𝑒

𝑄_{𝑐} (3)

**1.4.2 Battery Life Definition **

The most common definition of battery life is as cycle life. This is easy and
meaningful when the load history of the battery is regular, so that a “cycle” is always the
same. However, in HEVs, the battery is not cycled on a regular basis, because the current
history depends on the driving path. Thus, the definition of life as number of cycles would
imply the designation of a “standard” or “equivalent” cycle, which would lead to
non-intuitive results. For this reason, in this work the battery life L_{tot}is expressed as a
total amount of charge that can be drawn from the battery. The charge life of a battery can
be derived from the cycle life using the following equation [19]:

For example, for a 6.5 Ah battery,
𝐿_{𝐴ℎ}(𝐷𝑂𝐷 − 10%) = 5400𝑐𝑦𝑐𝑙𝑒𝑠 ∗ 10
100∗ (6.5𝐴ℎ) = 3510𝐴ℎ
𝐿_{𝐴ℎ}(𝐷𝑂𝐷 − 20%) = 2700𝑐𝑦𝑐𝑙𝑒𝑠 ∗ 20
100∗ (6.5𝐴ℎ) = 3510𝐴ℎ
𝐿𝐴ℎ(𝐷𝑂𝐷 − 30%) = 1500𝑐𝑦𝑐𝑙𝑒𝑠 ∗
30
100∗ (6.5𝐴ℎ) = 2925𝐴ℎ

**1.4.3 Efficiency **

A battery, as an electro-thermal system, encounters the same efficiency losses as all systems that deal with the laws of thermodynamics. When a battery is being discharged, the current seen at its terminals is downstream of all the electro-thermal losses encountered, starting from the charge migration from deep inside the plates, to the plate-electrolyte interface, through the electrolyte to the terminals, and out through wire of a certain gage. Therefore, to have the battery reach the same state of charge as before one started, one must put back more current than one pulled out.

Conventional wisdom (such that comes from mechanics and mechanic-oriented websites) states that automotive batteries should be recharged with 110% as much charge for the battery to reach the original state of charge. This efficiency that penalizes charging current from fully contributing to state of charge is called the Coulombic or calorimetric efficiency [43]. It is, however, sometimes neglected in computation if a reliable method to determine state of charge is not extant to determine this value empirically, and if it has not been provided by the manufacturer [7].

The efficiency will be

η=𝐸𝑑

𝐸_{𝑐} (5)
𝐸_{𝑑}: 𝐷𝑖𝑠𝑐ℎ𝑎𝑟𝑔𝑒𝑑 𝐸𝑛𝑒𝑟𝑔𝑦

**2. Literature Review **

**2.1 Reasons for aging **

Aging on cycling is often described as the result of degradation of active materials reversibility, especially the positive, coming from phase transformations during lithium insertion. This is beyond the scope of this paper to describe these mechanisms, which are extensively studied and published for many materials. In some cases, the fading rate may exhibit an inflexion point, where the capacity loss starts to increase, instead of decreasing [23]. When dismantling the cells, a large deposit of Li metal was observed, this was the reason for rapid capacity decay. In the same time, a strong increase in cell resistance is observed. There would be a specific point exhibiting a change in the slope of the capacity or resistance curves, probably when Li starts to plate significantly.

When induced, lithium plating itself will produce more deposit, and aggravates the phenomenon, which explains the increasing of capacity fading rate. Indeed, the electrode porosity is recognized as one of the first-order parameters controlling the capacity fade on cycling [24].

**2.2 Aging Effect **

The charging rate has obviously a strong influence on this behavior. Temperature decrease would accelerate the fading rate, lowering the limit at which the Li plating will occur, and for the same reasons increasing temperature in some limits would be beneficial. This is a tradeoff effect between lithium corrosion rate, which accelerates reduction of active area (negative effect of temperature), and concentration gradients producing high local current density (positive effect of temperature) [23].

**2.2.1 Electrolyte **

It is widely known from literature, that electrolyte decomposition and the corresponding formation of solid electrolyte interphase (SEI), is the dominant aging process in most graphite-based lithium-ion batteries during storage leading to capacity decline (due to loss of active lithium) and impedance rise (due to increase in film layer thickness). Theoretical derivations of the time dependency of the SEI growth rate are quite opposing [20]. Overcharging and over-discharging the battery leads generally to electrolyte decomposition. This results in a decreased electrolyte conductivity, which leads to an increase of internal resistance [27].

Figure 2 Changes at the anode/electrolyte interface

Changes at the electrode/electrolyte interface due to reactions of the anode with the electrolyte are considered by many researchers to be the major source for ageing of the anode. It is well known that lithium-ion battery anodes operate at voltages that are outside the electrochemical stability window of the electrolyte components. Hence, reductive electrolyte decomposition accompanied by irreversible consumption of lithium ions takes place at the electrode/electrolyte interface when the electrode is in the charged state. The decomposition products build up “protective layers” that cover the electrode’s surface. This process occurs mainly (but not exclusively) at the beginning of cycling, especially during the first cycle [2].

damage. In the model it was assumed that no NMP is emitted to the environment [17].

**2.2.3 Positive electrode (Anode) **

The anode is generally made of graphite coated on copper foil about 14 mm thick. In addition a binder is needed. As with the cathode, the LCA data used for the anode ingredients was found in the Ecoinvent database. For the anode made with water a styrene butadiene latex binder was used. It was approximated with ABS, acrylonitrile butadiene styrene, from the Ecoinvent database. [13]

Chemical reaction happens on the positive electrode:
For Charging:
LiFePO_{4}− 𝑥𝐿𝑖+_{− 𝑥𝑒}− _{→ 𝑥𝐹𝑒𝑃𝑂}
4+ (1 − 𝑥)𝐿𝑖𝐹𝑒𝑃𝑂4
For Discharging
FeP𝑂_{4}+ 𝑥𝐿𝑖+_{+ 𝑥𝑒}− _{→ 𝑥𝐿𝑖𝐹𝑒𝑃𝑂}
4+ (1 − 𝑥)𝐹𝑒𝑃𝑂4

An additional SEI formation mechanism results from insertion of lithium into graphite layers. This causes an increase of the lattice volume. The surface film can be stretched and even destroyed. This damage is repaired by a chemical reaction that irreversibly consumes lithium, but thereby battery capacity decreases. In the case of lithium metal negative electrodes, growth of dendrites at small discharge currents can be observed. This leads to an increase of self-discharge. The probability of internal short circuit becomes higher [27].

**2.3 Aging Models **

**2.3.1 Resistance Increasing in ECM **

Between the low-level chemical modeling and the input-output heuristic-level modeling exists a compromise. It is possible to understand the chemical processes in the battery, and approximate their effects as the behavior of a lumped-model network of higher-level physical systems. In this section, we review a number of ways to reduce complex chemical phenomena to well-understood and well-behaved electrical-level circuit elements in creating a model.

In [31], many of the short-time and long-time processes inside batteries are identified and modeled. Figure 5 both lists the major dynamic processes inside batteries, and shows typical time scales on which they operate. An appreciation of these scales will be very useful when creating and using battery models.

Figure 4 A listing of the major dynamic processes in batteries and their average time constants

domain-specific. The model proposed, however, is not directly intended to model these effects but instead the shorter-time processes of mass transport, electric double-layering and charge storage, and electromagnetic processes. The technique of electrochemical impedance spectroscopy (EIS) was used here to observe these processes. This technique is another major topic of ongoing research for it may yield not only excellent battery models but may also allow predictive estimation of the states of the battery with respect to aging and other extremely long-term effects (viz., [19]). The technique has excellent primers elsewhere ([32]), but a briefly, the technique involves performing a frequency sweep of a complex system to compute its complex impedances using the amplitude and phase differences of the input and output signals. These complex impedances are then fit to a number of possible circuit models using least-squares, etc.

Diffusion processes occur in the active mass, the porous electrode, and in free electrolyte. They can be modeled using RLC elements either as a series of T-circuit ladders, as shown in Figure 5 and whose mathematics can grow unwieldy, or can be lumped into a Warburg impedance.

Figure 5 The RLC equivalent circuit needed to model diffusion effects

On a faster level is the double-layer capacitive effect, which many models stop at. This useful idea derives from the fact that charge must move from the solid electrode to the liquid electrolyte by crossing a charge-free region. This naturally warrants a capacitive description. A single layer turns out to be overly simplistic, as generally more than one of these capacitive layers form side-by-side: one right at the electrode-electrolyte interface and another beyond it.

circuit parameters vary by state of charge and temperature, and even battery age and current levels. (The series element is an ohmic resistance, discussed shortly.) Additional effects happen in this range when an electrode is porous (to maximize surface area, as is the case in automotive lead-acid batteries). During the following modeling, the ECM will be discussed in detail, so I just give a general introduction here.

**2.3.2 Aging **

**Detecting **

**From **

**Electrochemical Impedance **

**Spectroscopy **

Electrochemical techniques are very helpful for evaluation of batteries and cells during charge and discharge, and in service, as the nature of chemical and electrochemical processes occurring in these devices may be determined. Both traditional and an accelerated screening test method are necessary to analyze and compare battery properties, to obtain kinetic information, and to predict the likelihood of failure [16]. EIS maintains a high potential for ‘on-the-fly’ onboard vehicle battery assessment since it is relatively fast. The process can eventually be used as an approximation for reserve capacity and aging assessment to aid in prediction of future battery performance.

**2.3.2.1 First Order Randle Model **

𝑖_{𝑐} =𝑑𝑉𝑐

𝑑𝑡 ∗ 𝐶1 (7) The total current in the circuit will be:

i = 𝑖_{𝐶}+ 𝑖_{𝑅} (8)
After the Laplace Transform, we can get the equation:

𝑉_{𝑐}(𝑠) = 𝑅1

1 + 𝐶_{1}∗ 𝑅_{1}∗ 𝑠∗ 𝐼(𝑠) (9)
So the final expression for the total circuit will be:

V(s) = I(s) ∗ (𝑅_{0}+ 𝑅1

1 + 𝐶_{1}∗ 𝑅_{1}∗ s) (10)
So the transfer function between current and the voltage would be:

Tranfer function = (𝑅_{0}+ 𝑅1
1 + 𝐶_{1}2_{∗ 𝑅}
12 ∗ w2
) + −𝐶1∗ 𝑅12∗ w
1 + 𝐶_{1}2_{∗ 𝑅}
12∗ w2
∗ 𝑖 (11)
Assume that:
x = 𝑅0+
𝑅_{1}
1 + 𝐶_{1}2_{∗ 𝑅}
12∗ w2
(12)
y = −𝐶1∗ 𝑅1
2_{∗ w}
1 + 𝐶_{1}2_{∗ 𝑅}
12∗ w2
(13)

The mathematic result of the model should be:

(x − 𝑅0)2+ 𝑦2 = 𝑅2 (14)

R = 𝑅1

√1 + 𝐶_{1}2_{∗ 𝑅}
12 ∗ 𝑤2

(15)

When we increase the frequency of the system, we can witness the decreasing of the radius, if the frequency reach infinite, the radius is 0, oppositely, if the frequency were 0, the radius become the maximum that is R1. With the frequency range from the negative infinite to the positive infinite, the plot will be as the follows:

Figure 7 mathematic model of the first order of the impedance

**2.3.2.2 First order with WARBURG impedance **

The Warburg impedance is defined as an electrical component by:

𝑍_{𝑤} = 1

𝜎 ∗ (𝑖 ∗ 𝑤)𝑝 (16)

Where T is the length or magnitude and p is the angle in the complex plane. If p is 0.5, then the equation changes to:

𝑍𝑤 =

1

𝜎 ∗ √𝑖 ∗ 𝑤 (17)

And the angle is 45°. T corresponds to the diffusion of charge based on the material thickness [12]. The characteristics of this kind of impedance can be read easily from the

-1 -0.5 0 0.5 1 1.5 2 -0.5 -0.4 -0.3 -0.2 -0.1 0 0.1 0.2 0.3 0.4 0.5 0 dB -20 dB -10 dB -6 dB -4 dB -2 dB 20 dB 10 dB 6 dB4 dB2 dB Nyquist Diagram Real Axis Im a g in a ry A x is

Figure 8 Nyquist diagram of the Warburg Impedance

Figure 9 Bode plot of the Warburg Impedance

0 0.5 1 1.5 2 2.5 0 0.5 1 1.5 2 2.5 real value -i m a g in e v a lu e

Nyquist of the Warburg Impedance

10-4 10-2 100 102 104 106 0 1 2 3 4

### Frequency

### A

### m

### p

### lit

### u

### d

### e

### Bode Plot of the Warburg Impedance

10-4 10-2 100 102 104 106 -60 -40 -20 0

### Frequency

### P

### h

### a

### s

### e

The equivalent circuit model would be as follows:

Figure 10 ECM with Warburg impedance

Because of the adding of the Warburg Impedance, the current on the branch of the resistance will be changed. The new current going through will be:

𝑖_{𝑅} = 𝑉𝑐

𝑅_{1} + 𝑍 (18)
The transfer function will be

TF = 𝑅0+
1
𝐶_{1}∗ 𝑠 +_{𝑅} 1
1+ (𝜎 ∗ 𝑠0.5)−1
(19)
s = w ∗ i and i0.5 _{=}20.5
2 ∗ (1 + i) (20)
The real part would be

Real = 𝑅1+
20.5
2 ∗ 𝜎 ∗ 𝑤0.5
(1 + 𝐶1∗ 𝑤
0.5
20.5_{∗ 𝜎)}
2
+ (𝐶1∗ 𝑅1∗ 𝑤 + 𝐶1∗ 𝑤
0.5
20.5_{∗ 𝜎)}
2+ 𝑅0 (21)

The imagine part would be

Imag =
𝐶_{1}∗ 𝑅_{1}2_{∗ 𝑤 +}𝐶1
𝜎2 +_{𝜎 ∗ (𝑤 ∗ 2)}1 0.5+2
0.5_{∗ 𝑤}0.5_{∗ 𝐶}
1∗ 𝑅1
𝜎
(1 + 𝐶_{1}∗_{2}_{0.5}𝑤0.5_{∗ 𝜎)}2+ (𝐶_{1}∗ 𝑅_{1}∗ 𝑤 + 𝐶_{1}∗_{2}_{0.5}𝑤0.5_{∗ 𝜎)}2
(22)
If we assume the 1

σ reaches a value very close to 0.Then the final result will be

**2.3.2.3 High orders with or without Warburg impedance **

Figure 11 Nyquist diagram of the Second order without Warburg Impedance For the orders which is larger than 1, the equation of the result will be like this

V(s) = I(s) ∗ (𝑅_{0}+ 𝑅1

1 + 𝑅_{1}∗ 𝐶_{1}∗ 𝑠+ ⋯ +

𝑅_{𝑛}

1 + 𝑅_{𝑛} ∗ 𝐶_{𝑛}∗ 𝑠) (30)
The n is the number of the orders will be modeled during the experiment. Actually, the
real number of orders will not be higher than 4.

-1 -0.5 0 0.5 1 1.5 2 2.5 3 -0.8 -0.6 -0.4 -0.2 0 0.2 0.4 0.6 0.8 Nyquist Diagram Real Axis Im a g in a ry A x is

**2.3.3 Calendar Aging Model **

For HEV, PHEV and EV passenger cars applications, the battery packs spend more than 90% of the time in the calendar mode. During the parking mode, no current intensity flows in the battery pack. Thus, two stress factors impact the battery lifetime during this mode namely the temperature (T) and the state of charge of the system (SOC). To quantify the impact of these two aging factors on power and capacity fade, a parametric study is performed to simulate a 10-year storage period in three different regions of the world.

Based on the above mentioned simulation results for power and capacity loss, management strategies can be discussed to mitigate the aging of the system during the parking mode. According to the model predictions, drastic reduction of aging could be achieved by storing the battery at low SOC and low temperature.

The following figure done by E. Prada, shows clearly the influence of the temperature and state of charge. After a 10-year storage period at 100% SOC, the capacity loss in Dubai is 25.5% whereas in Moscow the value is 11.5%. The second interesting simulation result is related to the impact of SOC. As can be observed in the figure, the higher the SOC, the higher the capacity loss. For the case of Dubai, between 10 and 35% SOC, the capacity loss varies strongly from 1% to 20%. From 35% to 100%, one can notice the presence of two plateaus corresponding to the shape of the thermodynamic potential of the graphite negative electrode [1]. For the first plateau between 35% and 70% SOC, the capacity loss is around 23%. For the second plateau, above 75% SOC, the capacity loss is around 25%.

Figure 12 Model predictions for the capacity loss after a 10-year storage period at different SOC for the three cities

Figure 14 SEI resistance increase predictions as a function of the SOC of storage in Dubai

Based on the abovementioned simulation results for power and capacity loss, management strategies can be discussed to mitigate the aging of the system during the parking mode. According to the model predictions, drastic reduction of aging could be achieved by storing the battery at low SOC and low temperature. This battery management strategy could have sense for PHEV and EV applications for instance.

This model is a helpful tool to shed light into possible mechanisms leading to the battery end-of-life and a promising candidate for simulation studies, design specification purposes and BMS applications.

**2.3.4 Cycle Life Aging Model **

**2.3.4.1 Capacitance Retention **

Constant current–constant voltage (CC–CV) charging and constant current (CC) discharging are the most common schemes for LIB cycle life performance tests. For practical use, LIBs are charged by a charger that usually adopts the CC–CV charging scheme [37]. It is well known that LIBs significantly deteriorate with deeper DOD [35-36]. Therefore, DOD is one of the most important parameters for cycle life testing of LIBs. DOD is usually defined as the ratio of the discharged capacity to the rated capacity, and LIBs are cycled using CC discharging, with which the discharged capacity is invariably constant in every charge–discharge cycle.

Figure 15 shows the typical discharge curve trend of cell 1 during capacitance measurement. As the number of cycles increased, the curve slope steepened because of aging. Because the voltage slope during CC discharging is inversely proportional to the capacitance (dV/dt = I/C), the resultant discharge curve trends reflect capacitance fade due to aging.

Figure 16 redraws the capacitance retention trends of battery as a function of the square root of the number of cycles. It is empirically accepted that the retention trends of LIBs can be linearly extrapolated using the square root of the number of cycles or testing time as the x-axis [38], [39], [40].

Figure 16 Capacitance retention trends as a function of square root of number of cycles.

The degradation Rate can be extrapolated by using:

𝐷_{𝑇} = 𝑑_{𝑇}∗ √𝑁 (23)

Experimental retention trends and extrapolation curves agreed well for all temperature conditions, indicating that the extrapolation using (5) can be used to predict cycle life performance of LIBs at a given temperature for alternative battery applications.

In accelerated stress tests for electrolytic capacitors and semiconductor devices, an Arrhenius model is generally used to express temperature dependence of life. The

The acceleration factor for every 10 ℃ increase, i.e.,α is defined as
α = (𝑇 − 𝑇𝑟𝑒𝑓
10 ) ∗ √exp (
𝐸_{𝑎}
𝑅 ∗ (
1
𝑇𝑟𝑒𝑓−
1
𝑇)) (25)

Figure 17 Arrhenius plot trends of cycles

Figure 17 shows the resultant Arrhenius plot trend at each cycling condition. The results showed good linearity in all conditions, implying that the degradation rate was dominated by the ambient temperature in alternative battery applications in which the cell temperatures are considered to be almost equal to the ambient temperatures because of negligible heat generated during cycling.

**2.3.4.2 Capacity Fade **

Capacity characterization data were used to quantify the capacity fade rate for the model development. As an example, Figure 18 shows the discharge curves obtained at a C/2 rate (after different number of cycles) for the cells cycled under the following conditions: A, 90% DOD, C/2, 0 ◦C; B, 90% DOD, C/2, 45 ◦C; and C, 90% DOD, C/2, 60 ◦C. As cells age upon cycling, the measured capacities decrease steadily, while the shape of discharge profiles remained unchanged. These cycle number dependent capacity loss data were collected for the cycle life model development. The functional form of the life

𝑄_{𝑙𝑜𝑠𝑠} = f (t, T, DOD, Rate) (26)
Where t is the cycling time, T is the test temperature, DOD is the depth-of-discharge,
and Rate is the discharge rate for the cycle testing.

At a given C-rate, cells cycled at DODs greater than 50% were shown to reach the defined end of life condition sooner than those cycled at lower DODs (<50%). After eliminating DOD, capacity fade can only be affected by time (t) and temperature (T). In this case, we adopt the following battery life model [33]:

𝑄𝑙𝑜𝑠𝑠 = 𝐵 ∗ 𝑒 −𝐸𝑎

𝑅∗𝑇 ∗ 𝑡𝑧 (27)

To determine the fitting parameters, we implemented a single step optimization
process using Equation 4 with a slight rearrangement of the terms. The graphical
representation of this method is shown in Fig. 6 where ln(𝑄_{𝑙𝑜𝑠𝑠}) + 𝐸_{𝑎}/RT is plotted as a
function of ln(A-h). The activation energy 𝐸_{𝑎}was obtained from the intercept values of
the best-fit nonlinear regression curves. Applying the experimental data from 15, 45 and
60 ◦C at C/2 discharge rates, 𝐸_{𝑎} was found to be close to 31,500 J/mol. Previous reports
have indicated that this square-root of time relationship with capacity fade represents the
irreversible capacity loss due to solid electrolyte interface (SEI) growth that consumes
active lithium and is often controlled by a diffusion process.

**2.3.5 Shepherd Empirical Model **

The simulation model, which predicts the charge-discharge phenomena, is that proposed by Shepherd. This model presents the relation between voltage, current and the battery state of Charge Q as follows:

In discharge (I<0): U(t) = 𝑈𝑑 − 𝑔𝑑 ∗ 𝐼 ∗ 𝑡 𝐶+ 𝑅𝑑∗ (1 + 𝑀𝑑∗ 𝐼 ∗ 𝑡 𝐶 ∗ (1 + 𝐶𝑑) − 𝐼 ∗ 𝑡) (28) In charge (I>0): U(t) = 𝑈𝑐− 𝑔𝑐 ∗ (1 − 𝐼 ∗ 𝑡 𝐶) + 𝑅𝑐∗ 𝐼 ∗ (1 + 𝑀𝑐∗ 𝐼 ∗ 𝑡 𝐶 ∗ (1 + 𝐶𝑐) − 𝐼 ∗ 𝑡) (29)

Where U is the battery output voltage, g is the coefficient with characterize∆U = f(Q), C the capacity, R the internal resistance, I the current, t the time, T the temperature, M the slope of the U=f(t, I, Q) characteristic, SOC the state of charge (1-(Q/C)), DOD the deep of discharge (Q/C) and c, d are the indices of charge and discharge, respectively.

Thus the obtained model of aging is the following in discharge:

𝐶𝑑 = −0.005 − 0.0012 ∗ 𝑡 (30)
𝑈_{𝑑} = (2.175 − 0.0001 ∗ 𝐷2_{) − 0.036 ∗ log(0.25 ∗ 𝑡 + 1) (31) }
𝑀_{𝑑} = 0.065 + 0.011 ∗ log(0.75 ∗ 𝑡 + 1) (32)
𝑔_{𝑑} = 0.210 + 0.0473 ∗ log(0.33 ∗ 𝑡 + 1) (33)
𝑅_{𝑑} = (0.0053 + 0.0008 ∗ 𝐷) ∗ 20 − 0.5 ∗ 𝐷
√(20 − 0.5 ∗ 𝐷)2_{− 𝑡}2 (34)
In charge:
𝐶_{𝐶} = 1.15 + 0.0004 ∗ 𝑡 ∗ (𝑡 + 30) (35)
𝑈_{𝑐} = (2.01 + 0.00013 ∗ 𝐷2_{) + 0.0266 ∗ 𝑡 ∗ log(𝑡 + 1) (36) }
𝑀_{𝐶} = 0.55 + 0.053 ∗ log(0.25 ∗ 𝑡 + 1) (37)
𝑔_{𝑐} = 0.25 − 0.078 ∗ 𝑙𝑜𝑔(0.125 ∗ 𝑡 + 1) (38)
−𝑡

model. It is easy to find the model predict correctly the trend of the voltage variation during charging and discharging.

Figure 20 Discharge Voltage Variation for 4 states of ageing

Moreover, he demonstrated how the battery aging affects all parameters of the Shepherd model. This variation is most remarkable with dynamic solicitations (in current and load consumption). However, in nominal functioning conditions, the aging affects slightly the output voltage and is not significant before the first year. To protect the battery from deep discharges and irreversible corrosion, the load request and the power consumption must be limited and controlled. To avoid deep discharge, the voltage output must be fixed in function of the discharge current. Finally, the battery regulator in insufficient to reduce aging consequences and thus must be assisted by an optimal management and monitoring of the PV plant.

**2.4 Battery Life Prediction from Aging **

Battery lifetime is one of the largest barriers preventing widespread adoption of lithium ion battery chemistries in automotive, as well as stationary applications. Sauer and Wenzl explain that all battery systems are affected by a wide range of aging processes in Comparison of different approaches for lifetime prediction of electrochemical systems [11]. They explain that many of these processes occur due to different stress factors and operating conditions imposed on the battery. Some of these factors include the number of charging cycles a battery has experienced, the battery state of charge at which cycling occurs, frequency of battery operation, and wide ranges of temperatures during operation[10]. For this project, we are not concerned with calendar aging, but with the aging that occurs as a result of the amp hour throughput experienced by the battery. In this paper, a large number of cells were aged across a wide range of conditions and the aging effects displayed by each battery were analyzed with respect to each battery’s experienced amp hour throughput. The experiments were designed to gather data that could be used to analyze the severity of capacity degradation while aging batteries in fringe areas of their operating regions. The methods represent procedures that can be used in real time to predict the remaining life of a battery, which is what this work hopes to accomplish.

**2.4.1 First Method (based on Resistance Growth)**

The first life prediction method calculated estimates for the predicted growth of internal resistance based directly on the local slope values identified using the resistance growth dynamic model. This was accomplished by utilizing a sliding window method similar to what was used when averaging calculated resistance values and identifying local slope values. The predicted resistance growth was determined by averaging a set of

unreasonable resistance growth predictions or those with a negative slope, which was possible if the lower growth estimate was calculated using the same method as the upper growth estimate by subtracting the standard deviation from the average growth rate [10].

Figure 24 Example of Life Prediction Using Method 1 at 3500 Amp Hours

By extrapolating the lines of predicted resistance growth to a threshold value of normalized resistance, a life prediction could be made in terms of amp hours. A threshold of 10% growth was chosen for the purpose of making life predictions simply for illustrative purposes, although other threshold values could be chosen. For Instance, because resistance growth is directly related to power loss, this threshold could be set so that life predictions would forecast the amp hours remaining in a battery pack’s life until it could no longer meet performance requirements in a vehicle. Each prediction was made at the battery age shown on the x-axis and included the mean predicted life, the lower life estimate based on the worst case, and the best expected life which was chosen to be the

Figure 25 Prediction of the life from the resistance

Although the life predictions made using method 1 provided some level of insight into the remaining life of the battery being tested, they were not ideal. The large error bars indicated low levels of precision and confidence in the estimates and the fact that the mean estimate never converged to a single value causes the accuracy of the method to be questioned. Although more trials were run using this method, their results were no better than those displayed in this example. For this reason, additional methods of life prediction were developed.

This cycle life prediction model suggests that capacitance retention,𝐶_{𝑇}, at a given
cycle number and a given temperature can be predicted by determining 𝛼 and 𝑑_{𝑟𝑒𝑓}.

Figure 26 shows the capacitance retention trends predicted by the derived cycle life prediction model. The experimental and predicted retention trends were in good agreement, verifying that the cycle life prediction model is appropriate for batteries in alternative battery applications [41].

Batteries were cycled under various cycling conditions for 5000 cycles. The resultant capacitance retention trends were mainly influenced by temperature, and other conditions such as DOD and charge voltage were found to have only minor effects on the degradation. The experimental retention trends could be extrapolated linearly with the square root of the number of cycles as the x-axis.

The cycle life prediction model was derived from the combination of extrapolation and acceleration factor. The experimental and predicted capacitance retention trends were in good agreement, verifying that the derived prediction model is appropriate for SCs in alternative battery applications.

(b) As a function of square root of number of cycles. Figure 26 Examples of cycle life prediction

**2.4.3 Third Method (based on capacity fade) **

As a result, the capacity loss life model is expressed as:
𝑄_{𝑙𝑜𝑠𝑠} = 30330 ∗ exp ( −31500

8.3145 ∗ 𝑇∗ 𝐴ℎ0.552) (41) Using the life model in Equation (11), we are able to simulate qualitatively the capacity fade under various conditions in Figure 27, simulations of the capacity fade at different temperatures are compared to experimental data. Overall, the life model appears to be in a general agreement with the experimental data. The model slightly underestimates capacity loss at 60 ℃and overestimates capacity loss at 45℃. Their results demonstrate that at the low rates, time and temperature are the two parameters that substantially affect capacity fade and that DOD has a negligible effect on capacity fade [34].

Figure 27 Simulation of cycle-life prediction model and experimental data

Consequently, their modeling results are consistent with the aging mechanism that the active lithium is consumed to repair and/or grow the SEI layer when the carbon anode is cracked due to anode degradation. In addition, there is also a C-rate effect. The Arrhenius law used in the model equation represents the kinetics of the chemical processes for the undesired side reactions such as for SEI formation. The inverse relationship of the magnitude of activation energy with the C-rate suggests that higher rates produce higher diffusion induced stress field [42] on the particles which accelerates the chemical processes that cause irreversible active lithium consumption. They have demonstrated that this rather simple life model represents qualitatively the experimental data for all the rates investigated. It is also recognized that the accuracy of the life model predictions at the high rates produce slightly more error than at the low rates. Overall, this generalized approach allows us to present quantitative projections of capacity fading behaviors for a wide range of cycling conditions [34].

**2.5 International Standard **

**2.5.1 Life Testing **

The reference test cycle shall be used to determine battery life. The battery shall be discharged until 80 % of its benchmark energy content is removed or until the end of the micro-cycle in which 80 % of the energy is removed. The battery shall then be recharged, with the recharge starting within 1 h of the end of discharge. When the recharge is complete, the discharge shall be started within 1 h. [4]

The start of discharge could be delayed in order to fit in with the normal working practices of the test laboratory. Every fifty cycles, the battery energy content shall be determined using the benchmark test cycle. It will establish the actual energy content of the battery and allow the measurement of other parameters. During this test, a continuous record of battery system voltage shall be made so that other battery system parameters may be determined. Moreover, the total number of micro-cycles, the total Wh removed and the total Wh returned shall be recorded and declared as the battery energy content at this stage of the life test program. [4]

The life test shall be terminated when the energy delivered falls to below 80 % of the reference energy content. The number of reference test cycles shall be recorded and declared as the battery life.

**2.5.2 Maximum allowable deviations **

The overall accuracy of controlled (or measured) values, relative to the specific (or actual) values, shall be within the following tolerances:

Switching between power levels in the micro-cycle shall be timed such that the mid-point of the transition occurs at the point allocated for the transition.

The total duration of each complete micro-cycle shall be 360 s ± 1 s. [4]

**Parameters ** **Range **

**Temperature ** ±2 °C

**Power ** ±2 % of required value

**Time ** ±1 % of required value

**Power slew rate ** 1 s from one value of steady power to the next

**2.5.3 Intended Use **

**Test ** **Intended use simulation ** **Requirements **

**Electrical test A ** Storage after partial use No leakage (NL)

No explosion (NE)

**Environmental tests B1 Transportation shock ** No leakage (NL)

No explosion (NE)
**Environmental tests B2 Transportation vibration ** No leakage (NL)

No explosion (NE)
**Climatic-temperature ** Climatic-temperature cycling No explosion (NE)

Table 3 Intended Use of Battery [3]

The international standard IEC 60086-5 shows the boundary condition of the electrical and mechanical test. For the reason that the battery will not be used only in stationary situation, we must consider the influence from the environment and climate. We should simulate different kinds of condition to make sure the battery can work in all the situations.

**2.5.4 Failure Modes **

A battery is conventionally considered to be dead if its available capacity drops below 80% of its nominal capacity (presumably when it was new). A failure mode usually has 2 effects:

1. Decrease in capacity, and

2. Decrease in power delivery due to internal resistance.

Considering that the experiment may encounter some unpredicted problems, the following situation in the Table 4 will be considered as a failure, and the data from this kind of tests would not be used:

Failure Modes Surface Corrosion of Negative Electrode Decrepitation of Alloy Particles

Loss of Water in the Electrolyte Crystalline Formation

Cell Reversal High Self Discharge Shorted Cells

**2.6 Capacity Fade result from small format batteries **

**2.6.1 Small Size Li-Fe battery **

The Figure 28 show the normalized capacity in different DOD from 10% to 90% of a small size LiFePO4 battery, the nominal capacity is 2.2Ah. We can read from the line of DOD of 90%, the end of life (80% of the capacity) will happen at the cycle number 800. At the end of life the total Ah throughput will be 800*90%*2.2Ah=1600Ah.

Figure 28 Capacity retention at 60 ◦C and a discharge rate of C/2 plotted as a function of cycle number, data shown for different DOD [34]

This observation is illustrated in Figure 28, where capacity retention as a function of cycle number at various DODs for the cells at 60 .C and C/2 rate is plotted. When plotted in this manner capacity fade appears to be a function of DOD. However, when

concluded that the DOD effect was not important for the conditions investigated. Thus, the DOD effect was not considered for formulating a model for at low discharge rates.

Figure 29 Capacity retention at 60 .C and a discharge rate of C/2 plotted as a function of time (days)

**2.6.2 LiCo2/C Battery **

In the Figure 30capacity may decline very rapidly after a first “normal” phase. When dismantling the cells described in Figure 30 after cycling, a large deposit of Li metal was observed, this was the reason for rapid capacity decay. In the same time, a strong increase in cell resistance is observed

Due to a reduction in charging capability of the cell, the degradation mechanism can be explained by the progressive clogging of the micropores of the negative electrode by the passivation layer growth. If this reaction is not stabilized enough, the reactions products (Li2CO3, alkyl-carbonates, polymers) will depose in the microposity, thus significantly reducing the active surface area.

When induced, lithium plating itself will produce more deposit, and aggravates the phenomenon, which explains the increasing of capacity fading rate. Indeed, the electrode porosity is recognized as one of the first-order parameters controlling the

behavior. Temperature decrease would accelerate the fading rate, lowering the limit at which the Li plating will occur, and for the same reasons increasing temperature in some limits would be beneficial. This is a tradeoff effect between lithium corrosion rate, which accelerates reduction of active area (negative effect of temperature), and concentration gradients producing high local current density (positive effect of temperature) [23].

Figure 30 Example of capacity evolutions during 100% DOD cycling. LiCoO2/graphite pouch cells, charge at C, discharge at C/2, 20 C).

Although each Li-ion chemistry may behave differently, there are few basic mechanisms, which may account for general aging phenomena in Li ion batteries. The most obvious is linked to the high reactivity of lithium from lithiated carbon, and

**2.6.3 10Ah LiFePO**

**4**

**-based Li-ion batteries **

Two types of large format (>10 Ah) LFP cells, denoted as “Cell L” and “Cell P”, were purchased from two manufacturers, respectively.

In the life cycle tests, Cell L was first characterized at 25 Celsius with a procedure comprises 10 cycles of charge–discharge regime at C/10 and 5 cycles with C/10 charge and C/2 discharge. Cell L was then subjected to 1 C/10 cycle and 100 cycles of C/10 charge and C/2 discharge regime at 60 Celsius. The end-of-charge (EOC) cutoff condition comprises a typical cutoff voltage at 4.2V and a capacity limit of 10 Ah. At the end of the life cycle test, 10 additional C/10 cycles were carried out at 60 Celsius. Cell P was tested using a different test plan and protocol. A C/10 cycle was conducted first, followed by four cycles of C/10 charge and C/2 discharge regime. Such a five-cycle regimewas repeated at 25 and 60 Celsius. The data and presentations used in the illustration and discussion in this paper are selected from representative cells in each type that are worth discussion or comparison. Therefore, the result generally reflects the behavior of each type of cells.

Figure 31 (a) Voltage.capacity curves for Cell L in the first 15 cycles at 25 Celsius. (b) Voltage.capacity curves for Cell P in the first 5 cycles at 25 Celsius.

Figure 31(a) displays the voltage vs. capacity curves in the first few cycles of Cell L at 25 Celsius. Little change was observed among the first 15 cycles. The cell delivered 11.35 Ah at C/10 and 11.14 Ah at C/2.

Figure 31 (b) shows similar curves in the first 5 cycles of Cell P. The cell delivered a higher capacity with 13.38 Ah at C/10 and 13.07 Ah at C/2. Although the shape of discharge curves appears similar, Cell P released more capacity in the

Figure 32 (a) Capacity loss with cycle number for both cells and (b) evolution of the V vs. Q curves for Cell L.

Figure 32 (a) presents capacity retention with cycle number for Cell L and P. In Cell P, the capacity loss was immediate and the cell lost 4% after 4 cycles. In Cell L, the capacity was stable for about 15 cycles before a quick degradation kicked in. Subsequently, the cell lost 37% of its capacity after 100 cycles. Figure 32(b) displays the progression of the discharge (voltage vs. capacity) curve with cycle number in Cell L at 60 Celsius. Although the plateau voltage did not show significant changes over cycling, the length of the plateau seems to have changed significantly.

regimes, it remains stable in the last 10 C/10 regimes. The stable retention in the last C/10 cycles suggests that at low rates, the cell can consistently deliver the capacity in accordance with the active material content remained in the cell. Overall, Cell L had lost about 45% of its capacity in the overall life cycle test through the C/2 regimes at 60 Celsius, according to the capacity determined by the last 10 C/10 cycles.

**3. Experimental Set-up **

**3.1 Test Bench for test **

Figure 34 Battery Test Bench

1: Battery 2: Power supply 3: Load

4: Data Acquisition System 5: Computer

This is the test bench for the battery and it can be divided into 5 parts: battery, power supply, load, data acquisition system and PC. The following figures (Figure 35 and Figure 36) show the hardware structure during the charging and discharging phase.

## 5

## 1

## 2

## 4

## 3

Figure 35 Connection During Charging

AO: Analog output Signal AI: Analog input Signal RC: Remote Control

With the application of the MATLAB, we can control all the electric components in the bench, and receive all the information of the battery. The boundary condition set in the program of the PC (Highest Voltage and Lowest Voltage of the Battery) will decide the critical time for shifting the phase. In the serial communication port (A/D convertor), we can set the sampling frequency and time-out to get the required data we want.

In the Charging phase, the computer set the current and voltage of the power supply by remote sensing. The load will measure the current going through and the temperature of air and heat sink. The data acquisition system will also record the battery temperature and the voltage of the battery continuously. At the same time, the DAQ will send the monitoring result to the PC.

Current Current Load DAQ Computer Power Supply Battery I, T_air, T_heatsink V,T_battery Monitoring RC

Figure 36 Connection During Discharging

During the discharging phase, most the monitoring procedure will be almost the same. But the power supply will be completely useless and we can switch off the power supply will the command. What should be pointing out is that the analog output signal should be decided carefully to control the discharged current.

Current Load DAQ Computer Battery I, T_air, T_heatsink V,T_battery Monitoring AO Current Control

**3.1.1 Battery Specification **

SINOPOLY LITHIUM ION BATTERY SPECIFICATIONS:

Figure 37 Battery model: TS-LFP60AHA(A) [25]

**Model ** **TS-LFP60AHA(A) **

**Nominal Capacity ** 60Ah,192Wh

**Nominal Voltage ** 3.2V

**Life Cycle ** 80%DOD ≥3000Times

70%DOD ≥4000Times

**Self-discharge Rate ** ≤3%

**Charge ** **Discharge **

**Cut-Off Voltage ** 4V 2.8V

**Standard Current ** 0.5C,30A 0.5C,30A

**Max Constant Current ** 3C,180A 3C,180A

**Max Impulse Current ** 20C,1200A 20C,1200A

**Operating Temperature ** −45𝑜𝐶 + 85𝑜𝐶 −45𝑜𝐶 + 85𝑜𝐶

Table 6 Electric parameters of charge and discharge

In the Table 5, we can read the nominal voltage 3.2V and the nominal capacity 60Ah. The related power will be the production of the two that is 192Wh. For different DOD, the cycling life will be different: Increasing DOD will lead the shrinkage of the life of the lithium battery. The self-discharge rate is very small (only 3%), so we do not need to consider the influence of self-discharge on the experiment. Table 6 shows the standard parameters, current limitation and operation temperature of this type of battery. All the data here are produced by the factory of the battery, so it can be treated as the reference of the following test.

Figure 41 LFP battery’s circulation charging and discharging curve under normal temperature

From Figure 38 to Figure 41, we can see different characteristics of the batteries. In the Figure 38, the voltage decreases rapidly at the beginning of the discharging, and then the trend becomes stabilized between 15Ah and 45Ah. After that, the voltage drops very quickly to the lowest point at 68 Ah. Figure 39 shows clearly the calendar aging of the battery during storage, we can find that the capacity decreases from 100% to 65% smoothly. The influence of the temperature can be read in the Figure 40, in high temperature environment, the voltage seems to be horizontal in a longer time than that of lower temperature.